Tải bản đầy đủ - 0 (trang)

3 Alternating hybrid algorithms: CNT growth by MD/fbMC

Theor Chem Acc (2013) 132:1320

state. The red atoms indicate the carbon atoms involved in the

formation of the new diamond 6-ring. Reproduced from [74] with

permission from the Royal Society of Chemistry

Fig. 3 Formation of a new diamond 6-ring from an adsorbed C-atom

and adsorbed C2H2 molecule as observed in a MD/MMC simulation.

a The initial conﬁguration, b–d intermediate states and e the ﬁnal

and electronic properties. However, these properties are

directly determined by their precise structure, thus necessitating very accurate control over the growth process. In

this case, atomistic simulations may provide the atomic

scale insight needed to understand how the growth process

might be controlled, and why speciﬁc structures are formed

for a given growth condition.

One very important factor during the growth is the phase

state of the nanocatalyst. Thus, we performed MD/fbMC

simulations, employing the Shibuta potential, to determine

the phase state of various Ni-nanoparticles as a function of

size and temperature [76]. In this work, the thermalization

was carried out using combined MD/fbMC simulations.

Analysis of the radial distribution of the atomic Lindemann

index revealed that that for the smallest clusters, a dynamic

coexistence process occurs. As illustrated in Fig. 4, surface

melting is observed for the larger particles. In all cases, a

signiﬁcant depression of the melting temperature relative to

the bulk was observed, due to the Gibbs–Thomson effect,

in agreement with the literature [77–79].

Subsequently, a number of combined MD/fbMC simulations were performed to study the growth of carbon

nanotubes based on the ReaxFF potential to gain an

atomic scale understanding in the actual growth process

[80–82]. In these simulations, rather conservative values

for D=2 ¼ 0:085Req [80] and D=2 ¼ 0:07Req [81, 82] in

the fbMC were chosen. The temperature was set to 1,000 K,

corresponding to a typical experimental growth temperature. After each MC cycle, new random velocities were

assigned to all atoms, and the simulation was continued

with constant temperature MD. Similar to Grein et al., the

impact and deposition of atoms (in this case C-atoms) on

the substrate (in this case a Ni-nanocluster) were followed

by MD, and the subsequent relaxation by fbMC. It was

found that the fbMC method results in healing of the carbon network that is formed by the continuous addition of

carbon atoms—a process in which high barriers must be

overcome. An example of this healing mechanism as

Reprinted from the journal

Fig. 4 Calculated radial distribution of the atomic Lindemann index

for a Ni244 cluster, for various temperatures, revealing a surface

melting mechanism. Reproduced from [15] with permission from the

American Chemical Society

observed in the fbMC is shown in Fig. 5. This then ﬁnally

leads to CNTs with very few defects, as illustrated in

Fig. 6, in contrast to what is typically observed in pure MD

growth simulations. Both metallic tubes [81] as well as

semi-conducting tubes [80] could be obtained. Furthermore, we also observed that the chirality of the tube may

change in the initial nucleation stage. It was found that this

is due to the incorporation of asymmetric defects, such as

so-called 5–7 defects [81]. Thus, these MD/fbMC simulations allow to gain an understanding of how the longer

timescale events may inﬂuence the growth process.

In another study, we used MD/fbMC simulations to

investigate how an electric ﬁeld may inﬂuence the growth

process. In agreement with the experiment [83, 84], SWNT

285

123

Theor Chem Acc (2013) 132:1320

simulations directly provide information about the relevant

processes complementary to the experiment.

5 Conclusion

In this contribution, we have presented a brief summary of

the main accelerated molecular dynamics techniques as

well as more a elaborate description of the various techniques for combining MD simulations with MC simulations, as an alternative to accelerated molecular dynamics

simulations for generating long system trajectories. Using

examples from the literature, it is shown that combined

MD/MC simulations may provide a dynamic picture of a

reactive system, including relaxation events which take

place on timescales typically beyond the reach of pure MD.

Essentially, we can distinguish between algorithms in

which some atoms are moved by MD and some by MC

(combined MD/MC method), algorithms in which the

atomic displacement prescription is in part deterministic

and in part stochastic (hybrid MD/MC method), and algorithm in which MD cycles alternate with MC cycles

(sequential MD/MC method).

Three representative examples from our own research

efforts were shown to demonstrate the applicability of MD/

MC simulations, viz. Cu adatom diffusion, UNCD growth

and CNT growth.

In addition to their ease of implementation and their

general applicability make these methods very attractive

for studying systems in which processes beyond the reach

of standard MD are important.

Fig. 5 Observed healing mechanism of the growing carbon network

during CNT growth. Reproduced from [81] with the permission of the

American Chemical Society

Fig. 6 Simulated SWNT

growth based on the MD/fbMC

technique, resulting in a SWNT

with (7, 7) chirality.

Reproduced from [81] with

permission from the American

Chemical Society

References

1. Frenkel D, Smit B (2001) Understanding molecular simulation:

from algorithms to applications. Academic Press, London

2. Cooke DJ, Elliott JA (2007) Atomistic simulations of calcite

nanoparticles and their interaction with water. J Chem Phys

127(10). Art no 104706

3. Khalilov U, Pourtois G, van Duin ACT, Neyts EC (2012) selflimiting oxidation in small-diameter Si nanowires. Chem Mater

24(11):2141–2147

4. Lu Y, Cheng H, Chen M (2012) A molecular dynamics examination of the relationship between self-diffusion and viscosity in

liquid metals. J Chem Phys 136(21). Art no 214505

5. Matsukuma M, Hamaguchi S (2008) Molecular dynamics simulation of microcrystalline Si deposition processes by silane

plasmas. Thin Solid Films 516(11):3443–3448

6. Neyts E, Bogaerts A, Gijbels R, Benedikt J, Van De Sanden M

(2004) Molecular dynamics simulations for the growth of diamond-like carbon ﬁlms from low kinetic energy species. Diam

Relat Mater13(10):1873–1881

7. Faccioli P, Lonardi A, Orland H (2010) Dominant reaction

pathways in protein folding: a direct validation against molecular

dynamics simulations. J Chem Phys 133(4). Art no 045104

Fig. 7 MD/fbMC simulation of vertically aligned SWNT growth by

applying an electric ﬁeld of 700 kV/cm [82]

alignment was observed if a (sufﬁciently strong) electric

ﬁeld was applied. This is shown in Fig. 7 for an electric

ﬁeld value of 700 kV/cm. These simulations shed a new

light on the underlying mechanism: we found that the

electric ﬁeld is primarily acting on the polar Ni–C bonds, at

the interface between the nickel nanocluster and the

growing SWNT. Thus, as at this interface the C-atoms are

slightly negative, while the Ni-atoms are slightly positive,

the carbon atoms experience both an oriented force, pulling

them toward the tip of the cluster, but are also subject to

random thermal diffusion. If the electric ﬁeld is sufﬁciently

strong, the directed migration dominates the random diffusion, an a vertically aligned SWNT emerges. Thus, these

123

286

Reprinted from the journal

Theor Chem Acc (2013) 132:1320

8. Rauf S, Sparks T, Ventzek PLG, Smirnov VV, Stengach AV,

Gaynullin KG, Pavlovsky VA (2007) A molecular dynamics

investigation of ﬂuorocarbon based layer-by-layer etching of

silicon and SiO2. J Appl Phys 101(3). Art no 033308

9. Gou F, Neyts E, Eckert M, Tinck S, Bogaerts A (2010) Molecular

dynamics simulations of Cl? etching on a Si(100) surface. J Appl

Phys 107(11):113305

10. Postawa Z, Czerwinski B, Szewczyk M, Smiley E, Winograd N,

Garrison B (2003) Enhancement of sputtering yields due to C-60

versus Ga bombardment of Ag{111} as explored by molecular

dynamics simulations. Anal Chem 75(17):4402–4407

11. Shen XJ, Xiao Y, Dong W, Yan XH, Busnengo HF (2012)

Molecular dynamics simulations based on reactive force-ﬁelds for

surface chemical reactions. Comput Theor Chem 990: 152–158

12. Servantie J, Gaspard P (2003) Methods of calculation of a friction

coefﬁcient: application to nanotubes. Phys Rev Lett 91(18). Art

no 185503

13. Thaulow C, Sen D, Buehler MJ (2011) Atomistic study of the

effect of crack tip ledges on the nucleation of dislocations in

silicon single crystals at elevated temperature. Mater Sci Eng A

Struct Mater Prop Microstruct Process 528(13–14):4357–4364

14. Shibuta Y (2012) Phase transition of metal nanowires conﬁned in

a low-dimensional nanospace. Chem Phys Lett 532:84–89

15. Neyts EC, Bogaerts A (2009) Numerical study of the sizedependent melting mechanisms of nickel nanoclusters. J Phys

Chem C 113(7):2771–2776

16. Dongare AM, Rajendran AM, LaMattina B, Zikry MA, Brenner

DW (2009) Atomic scale studies of spall behavior in nanocrystalline Cu. J Appl Phys 108(11):113518

17. Shaw DE, Maragakis P, Lindorff-Larsen K, Piana S, Dror RO,

Eastwood MP, Bank JA, Jumper JM, Salmon JK, Shan Y,

Wriggers W (2010) Atomic-level characterization of the structural dynamics of proteins. Science 330(6002):341–346

18. Metropolis N, Rosenbluth AW, Rosenbluth MN, Teller AH,

Teller E (1953) Equation of state calculations by fast computing

machines. J Chem Phys 21(6):1087

19. Kikuchi K, Yoshida M, Maekawa T, Watanabe H (1991)

Metropolis Monte–Carlo method as a numerical technique to solve

the Fokker-Planck equation. Chem Phys Lett 185(3–4): 335–338

20. Kikuchi K, Yoshida M, Maekawa T, Watanabe H (1992)

Metropolis Monte-Carlo method for Brownian dynamics simulation generalized to include hydrodynamic interactions. Chem

Phys Lett 196(1–2):57–61

21. Bortz AB, Kalos MH, Leibowitz JL (1975) A new algorithm for

Monte Carlo simulation of Ising spin systems. J Comput Phys

17:10–18

22. Netto A, Frenklach M (2005) Kinetic Monte Carlo simulations of

CVD diamond growth—interlay among growth, etching, and

migration. Diam Relat Mater 14(10):1630–1646

23. Henkelman G, Jonsson H (2001) Long time scale kinetic Monte

Carlo simulations without lattice approximation and predeﬁned

event table. J Chem Phys 115(21):9657–9666

24. Liu YH, Neyts E, Bogaerts A (2006) Monte Carlo method for

simulations of adsorbed atom diffusion on a surface. Diam Relat

Mater 15(10):1629–1635

25. Voter A, Montalenti F, Germann T (2002) Extending the time

scale in atomistic simulation of materials. Ann Rev Mater Res

32:321–346

26. Jonsson H, Mills G, Jacobsen KW (1998) Nudged elastic band

method for ﬁnding minimum energy paths of transitions. In:

Berne BJ, Ciccotti G, Coker DF (ed) Classical and quantum

dynamics in condensed phase simulations. World Scientiﬁc,

Singapore

27. Henkelman G, Jonsson H (1999) A dimer method for ﬁnding

saddle points on high dimensional potential surfaces using only

ﬁrst derivatives. J Chem Phys 111:7010–7022

Reprinted from the journal

28. Dellago C, Bolhuis PG, Csajka FS, Chandler D (1998) Transition

path sampling and the calculation of rate constants. J Chem Phys

108(5):1964–1977

29. Barkema GT, Mousseau N (1996) Event-based relaxation of

continuous disordered systems. Phys Rev Lett 77(21): 4358–4361

30. Allen RJ, Warren PB, ten Wolde PR (2005) Sampling rare

switching events in biochemical networks. Phys Rev Lett 94:

018104

31. Ren WE, Vanden-Eijnden E (2005) Finite temperature string

method for the study of rare events. J Phys Chem B 109:6668

32. Faradijan AK, Elber R (2004) Computing time scales from

reaction coordinates by milestoning. J Chem Phys 120:10880–

10889

33. Tironi IG, van Gunsteren WF (1994) A molecular-dynamics

simulation study of chloroform. Mol Phys 83(2): 381–403

34. Laio A, Parrinello M (2002) Escaping free-energy minima. Proc

Natl Acad Sci USA 99(20):12562–12566

35. Zwanzig RW (1954) High temperature equation of state by a

perturbation method. I. Nonpolar gases. J Chem Phys 22:1420–

1426

36. Torrie GM, Valleau JP (1977) Nonphysical sampling distributions in Monte Carlo free-energy estimation: umbrella sampling.

J Comput Phys 22(2):187–199

37. Darve E, Pohorille A (2001) Calculating free energies using

average force. J Chem Phys 115: 9169–9183

38. Leech J, Prins J, Hermans J (1996) SMD: Visual steering of

molecular dynamics for protein design. IEEE Comput Sci Eng

3:38–45

39. Sorensen M, Voter A (2000) Temperature-accelerated dynamics

for simulation of infrequent events. J Chem Phys 112(21):

9599–9606

40. Voter A (1997) Hyperdynamics: accelerated molecular dynamics

of infrequent events. Phys Rev Lett 78(20):3908–3911

41. Voter A (1998) Parallel replica method for dynamics of infrequent events. Phys Rev B Condens Matter 57(22): 13985–13988

42. Egelhoff WF, Jacob I (1998) Reﬂection high-energy electrondiffraction (RHEED) oscillations at 77 K. Phys Rev Lett 62(8):

921–924

43. Georgieva V, Voter AF, Bogaerts A (2011) Understanding the

surface diffusion processes during magnetron sputter-deposition

of complex oxide Mg-Al-O thin ﬁlms. Cryst Growth Des 11(6):

2553–2558

44. Fichthorn KA, Miron RA, Wang YS, Tiwary Y (2009) Accelerated molecular dynamics simulation of thin-ﬁlm growth with the

bond-boost method. J Phys Condens Matter 21(8):084212

45. Hamelberg D, Mongan J, McCammon JA (2004) Accelerated

molecular dynamics: a promising and efﬁcient simulation method

for biomolecules. J Chem Phys 120(24): 11919–11929

46. Uberuaga BP, Stuart SJ, Windl W, Masquelier MP, Voter AF

(2012) Fullerene and graphene formation from carbon nanotube

fragments. Comput Theor Chem 987(SI):115–121

47. Mees MJ, Pourtois G, Neyts EC, Thijsse BJ, Stesmans A (2012)

Uniform-acceptance force-bias Monte Carlo method with time

scale to study solid-state diffusion. Phys Rev B 85(13):134301

48. Laberge L, Tully J (2000) A rigorous procedure for combining

molecular dynamics and Monte Carlo simulation algorithms.

Chem Phys 260(1-2):183–191

49. Ribeiro AAST, de Alencastro RB (2012) Mixed Monte Carlo/

molecular dynamics simulations in explicit solvent. J Comput

Chem 33(8):901–905

50. Ulmschneider JP, Jorgensen WL (2003) Monte Carlo backbone

sampling for polypeptides with variable bond angles and dihedral

angles using concerted rotations and a Gaussian bias. J Chem

Phys 118(9):4261–4271

51. Leach AR (2001) Molecular modelling: principles and applications. Prentice Hall, Essex

287

123

Theor Chem Acc (2013) 132:1320

52. Bussi G, Donadio D, Parrinello M (2007) Canonical sampling

through velocity rescaling. J Chem Phys 126(1):014101

53. Forray C, Muthukumar M (2006) Langevin dynamics simulations

of genome packing in bacteriophage. Biophys J 91:25–41

54. Duane S, Kennedy A, Pendleton B, Roweth D (1987) Hybrid

Monte-Carlo. Phys Lett B 195(2):216–222

55. Mehlig B, Heermann D, Forrest B (1992) Hybrid Monte-Carlo

method for condensed-matter systems. Phys Rev B 45(2):

679–685

56. Clamp ME, Baker PG, Stirling CJ, Brass A (1994) Hybrid MonteCarlo—an efﬁcient algorithm for condensed matter simulation.

J Comput Chem 15(8):838–846

57. Brotz FA, Depablo JJ (1994) Hybrid Monte-Carlo simulation of

silica. Chem Eng Sci 49(17):3015–3031

58. Pangali C, Rao M, Berne B (1978) Novel Monte-Carlo scheme

for simulating water and aqueous-solutions. Chem Phys Lett

55(3):413–417

59. Rao M, Pangali C, Berne B (1979) Force bias Monte-Carlo

simulation of water—methodology, optimization and comparison

with molecular-dynamics. Mol Phys 37(6):1773–1798

60. Dereli G (1992) Stillinger-Weber type potentials in Monte-Carlo

simulation of amorphous-silicon. Mol Simul 8(6):351–360

61. Mezei M (1991) Distance-scaled force biased Monte Carlo simulation for solutions containing a strongly interacting solute. Mol

Simul 5:405–408

62. Timonova M, Groenewegen J, Thijsse BJ (2010) Modeling diffusion and phase transitions by a uniform-acceptance force-bias

Monte Carlo method. Phys Rev B 81(14):144107

63. Neyts EC, Thijsse BJ, Mees MJ, Bal KM, Pourtois G (2012)

Establishing uniform acceptance in force biased Monte Carlo

simulations. J Chem Theory Comput 8: 1865–1869

64. Rossky P, Doll J, Friedman H (1978) Brownian dynamics as

smart Monte-Carlo simulation. J Chem Phys 69(10): 4628–4633

65. Chiu S, Jakobsson E, Scott H (2001) Combined Monte Carlo and

molecular dynamics simulation of hydrated lipid-cholesterol lipid

bilayers at low cholesterol concentration. Biophys J 80(3):

1104–1114

66. Chiu S, Jakobsson E, Subramaniam S, Scott H (1999) Combined

Monte Carlo and molecular dynamics simulation of fully

hydrated dioleyl and palmitoyl-oleyl phosphatidylcholine lipid

bilayers. Biophys J 77(5):2462–2469

67. Jager HU, Belov AY (2003) ta-C deposition simulations: ﬁlm

properties and time-resolved dynamics of ﬁlm formation. Phys

Rev B 68(2):024201

68. Taguchi M, Hamaguchi S (2006) Molecular dynamics study on

Ar ion bombardment effects in amorphous Sio2 deposition processes. J Appl Phys 100(12):123305

69. Taguchi M, Hamaguchi S (2007) Md simulations of amorphous

Sio2 thin ﬁlm formation in reactive sputtering deposition processes. Thin Solid Films 515(12):4879–4882

70. Tavazza F, Nurminen L, Landau D, Kuronen A, Kaski K (2004)

Hybrid Monte Carlo-molecular dynamics algorithm for the study

123

71.

72.

73.

74.

75.

76.

77.

78.

79.

80.

81.

82.

83.

84.

288

of islands and step edges on semiconductor surfaces: application

to Si/Si(001). Phys Rev E 70(3, Part 2): 036701

Tiwary P, van de Walle A (2011) Hybrid deterministic and stochastic approach for efﬁcient atomistic simulations at long time

scales. Phys Rev B 84(10):100301

Grein C, Benedek R, Delarubia T (1996) Epitaxial growth simulation employing a combined molecular dynamics and Monte

Carlo approach. Comput Mater Sci 6(2):123–126

Eckert M, Mortet V, Zhang L, Neyts E, Verbeeck J, Haenen K,

Bogaerts A (2011) Theoretical investigation of grain size tuning

during prolonged bias-enhanced nucleation. Chem Mater 23(6):

1414–1423

Eckert M, Neyts E, Bogaerts A (2009) Modeling adatom surface

processes during crystal growth: a new implementation of the

metropolis Monte Carlo algorithm. CrystEngComm 11(8):1597–

1608

Eckert M, Neyts E, Bogaerts A (2010) Insights into the growth of

(ultra) nanocrystalline diamond by combined molecular dynamics

and Monte Carlo simulations. Cryst Growth Design 10(7):

3005–3021

Neyts EC, Khalilov U, Pourtois G, Van Duin ACT (2011)

Hyperthermal oxygen interacting with silicon surfaces: adsorption, implantation, and damage creation. J Phys Chem C 115(11):

4818–4823

Buffat P, Borel J (1976) Size effect on melting temperature of

gold particles. Phys Rev A 13(6):2287–2298

Jiang A, Awasthi N, Kolmogorov AN, Setyawan W, Borjesson A,

Bolton K, Harutyunyan AR, Curtarolo S (2007) Theoretical study

of the thermal behavior of free and alumina-supported Fe-C

nanoparticles. Phys Rev B 75(20):205426

Shibuta Y, Suzuki T (2010) Melting and solidiﬁcation point of

fcc-metal nanoparticles with respect to particle size: a molecular

dynamics study. Chem Phys Lett 498(4–6): 323–327

Neyts EC, Shibuta Y, Van Duin ACT, Bogaerts A (2010) Catalyzed growth of carbon nanotube with deﬁnable chirality by

hybrid molecular dynamics-force biased Monte Carlo simulations. ACS Nano 4(11): 6665–6672

Neyts EC, Van Duin ACT, Bogaerts A (2011) Changing chirality

during single-walled carbon nanotube growth: a reactive molecular dynamics/Monte Carlo study. J Am Chem Soc 133(43):

17225–17231

Neyts EC, Van Duin ACT, Bogaerts A (2012) Insights in the

plasma-assisted growth of carbon nanotubes through atomic scale

simulations: effect of electric ﬁeld. J Am Chem Soc 134(2):

1256–1260

Hatakeyama R, Kaneko T, Kato T, Li YF (2011) Plasma-synthesized single-walled carbon nanotubes and their applications.

J Phys D Appl Phys 44(17):174004

Kato T, Hatakeyama R (2006) Formation of freestanding singlewalled carbon nanotubes by plasma-enhanced CVD. Chem Vap

Depos 12(6):345–352

Reprinted from the journal

3 Alternating hybrid algorithms: CNT growth by MD/fbMC